Evaluating the Heat Resistance of Lead-Free Solder Containing
Evaluating the heat resistance of TA no.84 lead-free solder containing phosphorus 2008.2
1. Introduction weight increase in the same temperature region, which The use of lead-free solder has been steadily increasing indicates that solder oxidation, caused an exothermic as the regulation of hazardous substances by the RoHS reaction and weight gain. Directive expands globally. However, lead-free solder has Samples with added phosphorus repressed this oxidation a high melting temperature so soldering must be performed exothermic reaction, which indicate the oxidation repres- at a high temperature. This promotes the oxidation of sion effect of phosphorus. Furthermore, the differences in solder and weakens joint strength and connectivity. exothermic reaction and weight gain due to oxidation in The composition of solder is determined by considering the DTA curves show that the sample with 50ppm of various characteristics including workability, mechanical phosphorus more effectively repressed these reactions properties, and cost. However, it is crucial to examine than the sample with 25ppm. oxidation reaction differences caused by composition when Figure 2 shows the TG/DTA results for a solder sample considering working conditions. with 50ppm of phosphorus that was heated for one hour at In this brief, a Thermo Gravimetry/Differential Thermal 260℃. There was no change in the melting peak, which Analyzer (TG/DTA) is used to evaluate effect of additives suggests that a soldering temperature of 260℃ would not on the heat resistance of lead-free solder. change the characteristics of the solder. Furthermore, there was no exothermic reaction after melting, which 2. Measurement suggests that the oxidation repression effect of phosphorus The samples were Sn-3Ag-0.5Cu solder with various is long-lasting. amounts of phosphorous added to counteract oxidation 60 3.0 246℃ (Phosphorous content: 0, 25, 50ppm). 216℃ 40 2.5 The TG/DTA 6200 was used for measurements. 20 216℃ The measurement conditions were as follows; Sample 2.0 216℃ weight: 10mg, Atmosphere: Air, Temperature: room tem- 0 P： 0ppm 1.5 P： 25ppm perature to 450℃ at 20℃/min. A sample with 50ppm of DTA -20 P： 50ppm 1.0 TG ／ ％ phosphorus was heated for one hour at 260℃ before being DTA ／ μV TG measured under the conditions listed above. -40 0.5 -60 0.0 3. Results -80 -0.5 Figure １ shows the TG/DTA results for Sn-3Ag-0.5Cu 50 100 150 200 250 300 350 400 450 solder with amounts of different phosphorus. In the DTA Temp. ／ ℃ curves, all samples had a melting peak at 216℃. The Figure 1 TG/DTA results for Sn-3Ag-0.5Cu solder with added phosphorus phosphorus-free sample showed an exothermic peak im- mediately after melting (246℃). The TG curves showed a
Copyright © Hitachi High-Tech Science Corporation All rights reserved. ■ 1
20 2.0 216℃ 0 1.5
-20 DTA 1.0 TG ／ ％ DTA ／ μV TG -40 0.5
-80 -0.5 50 100 150 200 250 300 350 400 450 Temp ／ ℃ Figure 2 TG/DTA results for pre-heated solder (with 50 ppm of phosphorus)
4. Summary In this brief, a TG/DTA was used to measure lead-free solder containing different amounts of phosphorus. The results confirmed the presence of exothermic peaks and weight gain due to oxidation. The TG/DTA measurements performed in this brief can easily assess differences in the heat resistance of lead-free solder caused by additives to repress oxidation because the TG and DTA measurements are performed simultaneously. This ability makes TG/DTA an effective tool to investigate the relationship between soldering temperatures and oxidation degradation.
Acknowledgements We wish to thank Rikiya Katou of the Taguchi Laboratory at Senju Metal Industry, Co. for providing samples and advice.
References Application Brief TA no.74, Hitachi High-Tech Science Corporation (2003)
Copyright © Hitachi High-Tech Science Corporation All rights reserved. ■ 2